 
data_perb
 
_audit_creation_method            'SHELXL-2018/3'
_shelx_SHELXL_version_number      '2018/3'
_chemical_name_systematic         ?
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          ?
_chemical_formula_sum
 'Al2.27 H2 Ca0.97 Ce3.03 Fe1.16 Mg0.42 Mn0.15 O22 Si5' 
_chemical_formula_weight          1102.53

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mg'  'Mg'   0.0486   0.0363
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Al'  'Al'   0.0645   0.0514
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Si'  'Si'   0.0817   0.0704
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ca'  'Ca'   0.2262   0.3064
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mn'  'Mn'   0.3368   0.7283
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Fe'  'Fe'   0.3463   0.8444
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ce'  'Ce'  -0.2486   2.6331
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H'  'H'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       monoclinic
_space_group_IT_number            11
_space_group_name_H-M_alt         'P 21/m'
_space_group_name_Hall            '-P 2yb'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _space_group_symop_operation_xyz
 'x, y, z'
 '-x, y+1/2, -z'
 '-x, -y, -z'
 'x, -y-1/2, z'
 
_cell_length_a                    8.9458(2)
_cell_length_b                    5.72971(13)
_cell_length_c                    17.6192(3)
_cell_angle_alpha                 90
_cell_angle_beta                  115.9497(19)
_cell_angle_gamma                 90
_cell_volume                      812.06(3)
_cell_formula_units_Z             2
_cell_measurement_temperature     293(2)
_cell_measurement_reflns_used     7190
_cell_measurement_theta_min       3.3050
_cell_measurement_theta_max       32.3910
 
_exptl_crystal_description        'irregular'
_exptl_crystal_colour             'black'
_exptl_crystal_density_meas       ?
_exptl_crystal_density_method     ?
_exptl_crystal_density_diffrn     4.509          
_exptl_crystal_F_000              1023
_exptl_transmission_factor_min    ?
_exptl_transmission_factor_max    ?
_exptl_crystal_size_max           0.2014
_exptl_crystal_size_mid           0.1099
_exptl_crystal_size_min           0.0663
_exptl_absorpt_coefficient_mu     10.408
_shelx_estimated_absorpt_T_min    ?
_shelx_estimated_absorpt_T_max    ?
_exptl_absorpt_correction_type    'gaussian'
_exptl_absorpt_correction_T_min   0.247
_exptl_absorpt_correction_T_max   0.641
_exptl_absorpt_process_details    
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
Numerical absorption correction based on gaussian integration over
			a multifaceted crystal model
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details    ?
_diffrn_ambient_temperature       293(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_source                    'Enhance (Mo) X-ray Source'
_diffrn_measurement_device_type   'Xcalibur, Sapphire3'
_diffrn_measurement_method        'ω scans'
_diffrn_detector_area_resol_mean  16.0630
_diffrn_reflns_number             15902
_diffrn_reflns_av_unetI/netI      0.0267
_diffrn_reflns_av_R_equivalents   0.0398
_diffrn_reflns_limit_h_min        -12
_diffrn_reflns_limit_h_max        12
_diffrn_reflns_limit_k_min        -8
_diffrn_reflns_limit_k_max        8
_diffrn_reflns_limit_l_min        -25
_diffrn_reflns_limit_l_max        25
_diffrn_reflns_theta_min          2.707
_diffrn_reflns_theta_max          30.507
_diffrn_reflns_theta_full         25.242
_diffrn_measured_fraction_theta_max   0.999
_diffrn_measured_fraction_theta_full  0.998
_diffrn_reflns_Laue_measured_fraction_max    0.999
_diffrn_reflns_Laue_measured_fraction_full   0.998
_diffrn_reflns_point_group_measured_fraction_max   0.999
_diffrn_reflns_point_group_measured_fraction_full  0.998
_reflns_number_total              2696
_reflns_number_gt                 2532
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.000
_reflns_Friedel_fraction_max      .
_reflns_Friedel_fraction_full     .
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
 
_computing_data_collection        ?
_computing_cell_refinement        ?
_computing_data_reduction         ?
_computing_structure_solution     ?
_computing_structure_refinement 'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
_refine_special_details           ?
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0186P)²+5.3816P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      ?
_atom_sites_solution_secondary    ?
_atom_sites_solution_hydrogens    difmap
_refine_ls_hydrogen_treatment     refxyz
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        .
_refine_ls_number_reflns          2696
_refine_ls_number_parameters      202
_refine_ls_number_restraints      2
_refine_ls_R_factor_all           0.0401
_refine_ls_R_factor_gt            0.0355
_refine_ls_wR_factor_ref          0.0695
_refine_ls_wR_factor_gt           0.0679
_refine_ls_goodness_of_fit_ref    1.212
_refine_ls_restrained_S_all       1.211
_refine_ls_shift/su_max           0.000
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
Ce4 Ce 0.07678(5) 0.750000 0.16593(2) 0.01192(9) Uani 1 2 d S T P . .
Ce2 Ce 0.89196(5) 0.250000 0.25027(2) 0.01221(9) Uani 1 2 d S T P . .
Ce3 Ce 0.73868(6) 0.250000 0.00917(3) 0.02711(12) Uani 1 2 d S T P . .
Ce Ce 0.72989(17) 0.250000 0.40886(8) 0.0148(4) Uani 0.033(3) 2 d S T P . .
Ca Ca 0.72989(17) 0.250000 0.40886(8) 0.0148(4) Uani 0.967(3) 2 d S T P . .
Fe1 Fe 0.500000 0.500000 0.500000 0.0097(3) Uani 0.44 2 d S . P . .
Al1 Al 0.500000 0.500000 0.500000 0.0097(3) Uani 0.36 2 d S . P . .
Mg1 Mg 0.500000 0.500000 0.500000 0.0097(3) Uani 0.2 2 d S . P . .
Fe2 Fe 0.47953(15) 0.0000(2) 0.20518(8) 0.0087(4) Uani 0.048(6) 1 d . . P . .
Al2 Al 0.47953(15) 0.0000(2) 0.20518(8) 0.0087(4) Uani 0.952(6) 1 d . . P . .
Fe3 Fe 0.19082(13) 0.750000 0.37681(7) 0.0112(2) Uani 0.63 2 d S T P . .
Mg3 Mg 0.19082(13) 0.750000 0.37681(7) 0.0112(2) Uani 0.22 2 d S T P . .
Mn3 Mn 0.19082(13) 0.750000 0.37681(7) 0.0112(2) Uani 0.15 2 d S T P . .
Si1 Si 0.1588(2) 0.250000 0.47874(10) 0.0069(3) Uani 1 2 d S T P . .
Si2 Si 0.8015(2) 0.750000 0.33460(11) 0.0071(3) Uani 1 2 d S T P . .
Si3 Si 0.3027(2) 0.250000 0.31192(10) 0.0066(3) Uani 1 2 d S T P . .
Si4 Si 0.6692(2) 0.750000 0.10312(11) 0.0093(3) Uani 1 2 d S T P . .
Si5 Si 0.1548(2) 0.250000 0.07854(11) 0.0073(3) Uani 1 2 d S T P . .
O1 O 0.2623(4) 0.4899(6) 0.4828(2) 0.0135(7) Uani 1 1 d . . . . .
O2 O 0.1781(4) 0.4739(6) 0.2900(2) 0.0112(6) Uani 1 1 d . . . . .
O3 O 0.6911(4) 0.9861(6) 0.2991(2) 0.0116(6) Uani 1 1 d . . . . .
O4 O 0.4389(6) 0.750000 0.4225(3) 0.0131(9) Uani 1 2 d S T P . .
O5 O 0.4494(5) 0.250000 0.4111(3) 0.0112(9) Uani 1 2 d S T P . .
O6 O 0.4145(6) 0.250000 0.2585(3) 0.0099(9) Uani 1 2 d S T P . .
O7 O -0.0173(6) 0.250000 0.3981(3) 0.0131(9) Uani 1 2 d S T P . .
O8 O 0.9488(6) 0.750000 0.3066(3) 0.0217(12) Uani 1 2 d S T P . .
O9 O 0.8759(6) 0.750000 0.4374(3) 0.0198(11) Uani 1 2 d S T P . .
O10 O 0.5586(6) 0.250000 0.1633(3) 0.0105(9) Uani 1 2 d DS T P . .
H1 H 0.512(9) 0.250000 0.1097(7) 0.013 Uiso 1 2 d DS U P . .
O11 O 0.4006(5) 0.750000 0.2478(3) 0.0085(8) Uani 1 2 d DS T P . .
H2 H 0.418(10) 0.750000 0.2993(16) 0.010 Uiso 1 2 d DS U P . .
O12 O 0.5390(5) 0.750000 0.1478(3) 0.0106(9) Uani 1 2 d S T P . .
O13 O 0.2671(4) 0.4882(6) 0.1100(2) 0.0122(6) Uani 1 1 d . . . . .
O14 O 0.7926(4) -0.0267(6) 0.1316(2) 0.0164(7) Uani 1 1 d . . . . .
O15 O 0.5521(8) 0.6817(12) 0.0046(4) 0.0158(15) Uani 0.5 1 d . . P . .
O16 O 0.0611(8) 0.250000 -0.0219(3) 0.0340(15) Uani 1 2 d S T P . .
O17 O 0.0232(6) 0.250000 0.1176(3) 0.0217(12) Uani 1 2 d S T P . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
Ce4 O16 2.285(5) 3_565 ?
Ce4 O2 2.524(3) 4_575 ?
Ce4 O2 2.524(3) . ?
Ce4 O11 2.611(4) . ?
Ce4 O14 2.669(3) 4_465 ?
Ce4 O14 2.669(3) 1_465 ?
Ce4 O13 2.754(3) . ?
Ce4 O13 2.754(3) 4_575 ?
Ce4 O17 2.9675(14) . ?
Ce4 O17 2.9675(14) 1_565 ?
Ce4 Si4 3.3148(18) 1_455 ?
Ce4 Fe3 3.3954(11) . ?
Ce2 O7 2.365(5) 1_655 ?
Ce2 O14 2.460(4) 4_565 ?
Ce2 O14 2.460(4) . ?
Ce2 O2 2.668(3) 1_655 ?
Ce2 O2 2.668(3) 4_665 ?
Ce2 O10 2.691(4) . ?
Ce2 O3 2.758(3) 1_545 ?
Ce2 O3 2.758(3) 4_575 ?
Ce2 Si3 3.3451(17) 1_655 ?
Ce2 Si2 3.4817(10) 1_545 ?
Ce2 Si2 3.4817(10) . ?
Ce3 O17 2.423(5) 1_655 ?
Ce3 O15 2.535(7) 2_645 ?
Ce3 O15 2.535(7) 3_665 ?
Ce3 O14 2.547(4) 4_565 ?
Ce3 O14 2.547(4) . ?
Ce3 O13 2.563(3) 2_645 ?
Ce3 O13 2.563(3) 3_665 ?
Ce3 O12 2.794(5) 3_665 ?
Ce3 O15 2.965(7) . ?
Ce3 O15 2.965(7) 4_565 ?
Ce3 Si4 3.3031(18) 3_665 ?
Ce3 Si5 3.3716(17) 1_655 ?
Ca O7 2.351(5) 1_655 ?
Ca O3 2.358(3) 1_545 ?
Ca O3 2.358(3) 4_575 ?
Ca O1 2.398(4) 3_666 ?
Ca O1 2.398(4) 2_646 ?
Ca O5 2.527(5) . ?
Ca O6 2.905(5) . ?
Ca O9 3.097(2) . ?
Ca O9 3.097(2) 1_545 ?
Ca Si2 3.3262(11) . ?
Ca Si2 3.3262(11) 1_545 ?
Ca Si1 3.3757(11) 3_666 ?
Fe1 O4 1.887(3) . ?
Fe1 O4 1.887(3) 3_666 ?
Fe1 O1 2.014(3) . ?
Fe1 O1 2.014(3) 3_666 ?
Fe1 O5 2.023(3) . ?
Fe1 O5 2.023(3) 3_666 ?
Fe1 Fe1 2.86485(6) 2_656 ?
Fe1 Fe1 2.86485(6) 2_646 ?
Fe2 O10 1.885(3) . ?
Fe2 O11 1.892(3) 1_545 ?
Fe2 O3 1.894(3) 1_545 ?
Fe2 O13 1.907(3) 4_565 ?
Fe2 O6 1.937(3) . ?
Fe2 O12 1.957(3) 1_545 ?
Fe2 Fe2 2.864(3) 4 ?
Fe2 Fe2 2.865(3) 4_565 ?
Fe3 O8 1.968(5) 1_455 ?
Fe3 O4 2.002(5) . ?
Fe3 O2 2.169(3) . ?
Fe3 O2 2.169(3) 4_575 ?
Fe3 O1 2.253(4) . ?
Fe3 O1 2.253(4) 4_575 ?
Si1 O7 1.595(5) . ?
Si1 O9 1.638(5) 3_666 ?
Si1 O1 1.641(3) 4_565 ?
Si1 O1 1.641(3) . ?
Si2 O8 1.596(5) . ?
Si2 O3 1.630(3) 4_575 ?
Si2 O3 1.630(3) . ?
Si2 O9 1.633(5) . ?
Si3 O2 1.631(3) . ?
Si3 O2 1.631(3) 4_565 ?
Si3 O6 1.646(5) . ?
Si3 O5 1.663(5) . ?
Si4 O14 1.619(4) 1_565 ?
Si4 O14 1.619(4) 4_565 ?
Si4 O15 1.635(6) 4_575 ?
Si4 O15 1.635(6) . ?
Si4 O12 1.667(5) . ?
Si5 O16 1.592(5) . ?
Si5 O17 1.602(5) . ?
Si5 O13 1.641(3) 4_565 ?
Si5 O13 1.641(3) . ?
O10 H1 0.850(10) . ?
O11 H2 0.850(10) . ?
O15 O15 0.783(13) 4_575 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O16 Ce4 O2 140.95(8) 3_565 4_575 ?
O16 Ce4 O2 140.95(8) 3_565 . ?
O2 Ce4 O2 77.65(15) 4_575 . ?
O16 Ce4 O11 122.9(2) 3_565 . ?
O2 Ce4 O11 68.30(10) 4_575 . ?
O2 Ce4 O11 68.30(10) . . ?
O16 Ce4 O14 75.56(17) 3_565 4_465 ?
O2 Ce4 O14 116.25(10) 4_575 4_465 ?
O2 Ce4 O14 80.86(11) . 4_465 ?
O11 Ce4 O14 147.35(9) . 4_465 ?
O16 Ce4 O14 75.56(17) 3_565 1_465 ?
O2 Ce4 O14 80.86(11) 4_575 1_465 ?
O2 Ce4 O14 116.25(10) . 1_465 ?
O11 Ce4 O14 147.35(9) . 1_465 ?
O14 Ce4 O14 57.29(15) 4_465 1_465 ?
O16 Ce4 O13 73.78(16) 3_565 . ?
O2 Ce4 O13 127.39(10) 4_575 . ?
O2 Ce4 O13 85.67(10) . . ?
O11 Ce4 O13 59.18(10) . . ?
O14 Ce4 O13 109.55(10) 4_465 . ?
O14 Ce4 O13 148.95(10) 1_465 . ?
O16 Ce4 O13 73.77(16) 3_565 4_575 ?
O2 Ce4 O13 85.67(10) 4_575 4_575 ?
O2 Ce4 O13 127.39(10) . 4_575 ?
O11 Ce4 O13 59.18(10) . 4_575 ?
O14 Ce4 O13 148.95(10) 4_465 4_575 ?
O14 Ce4 O13 109.55(10) 1_465 4_575 ?
O13 Ce4 O13 65.99(14) . 4_575 ?
O16 Ce4 O17 74.94(10) 3_565 . ?
O2 Ce4 O17 143.68(12) 4_575 . ?
O2 Ce4 O17 66.12(12) . . ?
O11 Ce4 O17 99.18(10) . . ?
O14 Ce4 O17 56.91(12) 4_465 . ?
O14 Ce4 O17 112.31(13) 1_465 . ?
O13 Ce4 O17 54.48(12) . . ?
O13 Ce4 O17 118.06(12) 4_575 . ?
O16 Ce4 O17 74.94(10) 3_565 1_565 ?
O2 Ce4 O17 66.12(12) 4_575 1_565 ?
O2 Ce4 O17 143.68(12) . 1_565 ?
O11 Ce4 O17 99.18(10) . 1_565 ?
O14 Ce4 O17 112.31(12) 4_465 1_565 ?
O14 Ce4 O17 56.91(12) 1_465 1_565 ?
O13 Ce4 O17 118.06(12) . 1_565 ?
O13 Ce4 O17 54.48(12) 4_575 1_565 ?
O17 Ce4 O17 149.8(2) . 1_565 ?
O16 Ce4 Si4 69.45(18) 3_565 1_455 ?
O2 Ce4 Si4 102.40(8) 4_575 1_455 ?
O2 Ce4 Si4 102.40(8) . 1_455 ?
O11 Ce4 Si4 167.66(10) . 1_455 ?
O14 Ce4 Si4 28.90(8) 4_465 1_455 ?
O14 Ce4 Si4 28.90(8) 1_465 1_455 ?
O13 Ce4 Si4 129.97(7) . 1_455 ?
O13 Ce4 Si4 129.97(7) 4_575 1_455 ?
O17 Ce4 Si4 83.59(10) . 1_455 ?
O17 Ce4 Si4 83.59(10) 1_565 1_455 ?
O16 Ce4 Fe3 166.64(18) 3_565 . ?
O2 Ce4 Fe3 39.66(8) 4_575 . ?
O2 Ce4 Fe3 39.66(8) . . ?
O11 Ce4 Fe3 70.47(10) . . ?
O14 Ce4 Fe3 92.77(8) 4_465 . ?
O14 Ce4 Fe3 92.77(8) 1_465 . ?
O13 Ce4 Fe3 117.04(7) . . ?
O13 Ce4 Fe3 117.04(7) 4_575 . ?
O17 Ce4 Fe3 104.34(10) . . ?
O17 Ce4 Fe3 104.34(10) 1_565 . ?
Si4 Ce4 Fe3 97.19(4) 1_455 . ?
O7 Ce2 O14 139.33(9) 1_655 4_565 ?
O7 Ce2 O14 139.33(9) 1_655 . ?
O14 Ce2 O14 80.28(17) 4_565 . ?
O7 Ce2 O2 83.32(12) 1_655 1_655 ?
O14 Ce2 O2 82.04(11) 4_565 1_655 ?
O14 Ce2 O2 118.78(10) . 1_655 ?
O7 Ce2 O2 83.32(12) 1_655 4_665 ?
O14 Ce2 O2 118.77(10) 4_565 4_665 ?
O14 Ce2 O2 82.04(10) . 4_665 ?
O2 Ce2 O2 57.47(14) 1_655 4_665 ?
O7 Ce2 O10 112.79(15) 1_655 . ?
O14 Ce2 O10 67.53(10) 4_565 . ?
O14 Ce2 O10 67.53(10) . . ?
O2 Ce2 O10 147.81(8) 1_655 . ?
O2 Ce2 O10 147.81(8) 4_665 . ?
O7 Ce2 O3 67.23(11) 1_655 1_545 ?
O14 Ce2 O3 125.17(10) 4_565 1_545 ?
O14 Ce2 O3 82.48(10) . 1_545 ?
O2 Ce2 O3 149.64(10) 1_655 1_545 ?
O2 Ce2 O3 109.62(10) 4_665 1_545 ?
O10 Ce2 O3 57.76(10) . 1_545 ?
O7 Ce2 O3 67.23(11) 1_655 4_575 ?
O14 Ce2 O3 82.48(10) 4_565 4_575 ?
O14 Ce2 O3 125.17(10) . 4_575 ?
O2 Ce2 O3 109.62(10) 1_655 4_575 ?
O2 Ce2 O3 149.64(10) 4_665 4_575 ?
O10 Ce2 O3 57.76(10) . 4_575 ?
O3 Ce2 O3 66.50(14) 1_545 4_575 ?
O7 Ce2 Si3 81.00(12) 1_655 1_655 ?
O14 Ce2 Si3 102.31(8) 4_565 1_655 ?
O14 Ce2 Si3 102.31(8) . 1_655 ?
O2 Ce2 Si3 28.76(7) 1_655 1_655 ?
O2 Ce2 Si3 28.76(7) 4_665 1_655 ?
O10 Ce2 Si3 166.20(10) . 1_655 ?
O3 Ce2 Si3 132.20(7) 1_545 1_655 ?
O3 Ce2 Si3 132.20(7) 4_575 1_655 ?
O7 Ce2 Si2 64.01(5) 1_655 1_545 ?
O14 Ce2 Si2 145.91(9) 4_565 1_545 ?
O14 Ce2 Si2 76.54(9) . 1_545 ?
O2 Ce2 Si2 131.23(7) 1_655 1_545 ?
O2 Ce2 Si2 82.41(8) 4_665 1_545 ?
O10 Ce2 Si2 80.57(6) . 1_545 ?
O3 Ce2 Si2 27.26(7) 1_545 1_545 ?
O3 Ce2 Si2 90.76(7) 4_575 1_545 ?
Si3 Ce2 Si2 106.79(3) 1_655 1_545 ?
O7 Ce2 Si2 64.01(5) 1_655 . ?
O14 Ce2 Si2 76.54(9) 4_565 . ?
O14 Ce2 Si2 145.91(9) . . ?
O2 Ce2 Si2 82.41(8) 1_655 . ?
O2 Ce2 Si2 131.23(7) 4_665 . ?
O10 Ce2 Si2 80.57(6) . . ?
O3 Ce2 Si2 90.76(7) 1_545 . ?
O3 Ce2 Si2 27.25(7) 4_575 . ?
Si3 Ce2 Si2 106.79(3) 1_655 . ?
Si2 Ce2 Si2 110.74(5) 1_545 . ?
O17 Ce3 O15 139.06(18) 1_655 2_645 ?
O17 Ce3 O15 139.06(18) 1_655 3_665 ?
O15 Ce3 O15 17.8(3) 2_645 3_665 ?
O17 Ce3 O14 65.69(12) 1_655 4_565 ?
O15 Ce3 O14 89.03(17) 2_645 4_565 ?
O15 Ce3 O14 77.93(16) 3_665 4_565 ?
O17 Ce3 O14 65.69(12) 1_655 . ?
O15 Ce3 O14 77.93(16) 2_645 . ?
O15 Ce3 O14 89.03(16) 3_665 . ?
O14 Ce3 O14 76.99(16) 4_565 . ?
O17 Ce3 O13 106.46(12) 1_655 2_645 ?
O15 Ce3 O13 100.33(16) 2_645 2_645 ?
O15 Ce3 O13 111.10(16) 3_665 2_645 ?
O14 Ce3 O13 170.64(10) 4_565 2_645 ?
O14 Ce3 O13 104.96(11) . 2_645 ?
O17 Ce3 O13 106.46(12) 1_655 3_665 ?
O15 Ce3 O13 111.10(16) 2_645 3_665 ?
O15 Ce3 O13 100.33(16) 3_665 3_665 ?
O14 Ce3 O13 104.96(11) 4_565 3_665 ?
O14 Ce3 O13 170.64(10) . 3_665 ?
O13 Ce3 O13 71.64(15) 2_645 3_665 ?
O17 Ce3 O12 162.26(15) 1_655 3_665 ?
O15 Ce3 O12 58.30(17) 2_645 3_665 ?
O15 Ce3 O12 58.30(17) 3_665 3_665 ?
O14 Ce3 O12 126.50(10) 4_565 3_665 ?
O14 Ce3 O12 126.50(10) . 3_665 ?
O13 Ce3 O12 59.91(10) 2_645 3_665 ?
O13 Ce3 O12 59.91(10) 3_665 3_665 ?
O17 Ce3 O15 113.96(13) 1_655 . ?
O15 Ce3 O15 65.44(11) 2_645 . ?
O15 Ce3 O15 47.7(3) 3_665 . ?
O14 Ce3 O15 53.09(14) 4_565 . ?
O14 Ce3 O15 115.97(15) . . ?
O13 Ce3 O15 131.04(14) 2_645 . ?
O13 Ce3 O15 71.35(15) 3_665 . ?
O12 Ce3 O15 74.15(13) 3_665 . ?
O17 Ce3 O15 113.96(13) 1_655 4_565 ?
O15 Ce3 O15 47.7(3) 2_645 4_565 ?
O15 Ce3 O15 65.44(11) 3_665 4_565 ?
O14 Ce3 O15 115.97(15) 4_565 4_565 ?
O14 Ce3 O15 53.09(14) . 4_565 ?
O13 Ce3 O15 71.35(15) 2_645 4_565 ?
O13 Ce3 O15 131.04(14) 3_665 4_565 ?
O12 Ce3 O15 74.15(13) 3_665 4_565 ?
O15 Ce3 O15 113.1(3) . 4_565 ?
O17 Ce3 Si4 167.46(13) 1_655 3_665 ?
O15 Ce3 Si4 28.88(14) 2_645 3_665 ?
O15 Ce3 Si4 28.88(14) 3_665 3_665 ?
O14 Ce3 Si4 104.91(8) 4_565 3_665 ?
O14 Ce3 Si4 104.91(8) . 3_665 ?
O13 Ce3 Si4 83.59(8) 2_645 3_665 ?
O13 Ce3 Si4 83.59(8) 3_665 3_665 ?
O12 Ce3 Si4 30.28(10) 3_665 3_665 ?
O15 Ce3 Si4 61.48(12) . 3_665 ?
O15 Ce3 Si4 61.48(12) 4_565 3_665 ?
O17 Ce3 Si5 26.10(12) 1_655 1_655 ?
O15 Ce3 Si5 163.44(14) 2_645 1_655 ?
O15 Ce3 Si5 163.44(14) 3_665 1_655 ?
O14 Ce3 Si5 85.60(8) 4_565 1_655 ?
O14 Ce3 Si5 85.60(8) . 1_655 ?
O13 Ce3 Si5 85.43(8) 2_645 1_655 ?
O13 Ce3 Si5 85.43(8) 3_665 1_655 ?
O12 Ce3 Si5 136.16(10) 3_665 1_655 ?
O15 Ce3 Si5 121.93(12) . 1_655 ?
O15 Ce3 Si5 121.93(12) 4_565 1_655 ?
Si4 Ce3 Si5 166.44(5) 3_665 1_655 ?
O7 Ca O3 74.64(12) 1_655 1_545 ?
O7 Ca O3 74.64(12) 1_655 4_575 ?
O3 Ca O3 79.76(17) 1_545 4_575 ?
O7 Ca O1 111.72(12) 1_655 3_666 ?
O3 Ca O1 173.64(13) 1_545 3_666 ?
O3 Ca O1 101.35(12) 4_575 3_666 ?
O7 Ca O1 111.72(12) 1_655 2_646 ?
O3 Ca O1 101.35(12) 1_545 2_646 ?
O3 Ca O1 173.64(13) 4_575 2_646 ?
O1 Ca O1 76.86(17) 3_666 2_646 ?
O7 Ca O5 176.62(17) 1_655 . ?
O3 Ca O5 102.83(12) 1_545 . ?
O3 Ca O5 102.83(12) 4_575 . ?
O1 Ca O5 70.81(11) 3_666 . ?
O1 Ca O5 70.81(11) 2_646 . ?
O7 Ca O6 120.74(15) 1_655 . ?
O3 Ca O6 61.08(10) 1_545 . ?
O3 Ca O6 61.08(10) 4_575 . ?
O1 Ca O6 113.85(11) 3_666 . ?
O1 Ca O6 113.85(11) 2_646 . ?
O5 Ca O6 55.88(14) . . ?
O7 Ca O9 70.16(10) 1_655 . ?
O3 Ca O9 128.78(13) 1_545 . ?
O3 Ca O9 55.96(12) 4_575 . ?
O1 Ca O9 55.43(12) 3_666 . ?
O1 Ca O9 125.62(13) 2_646 . ?
O5 Ca O9 110.41(10) . . ?
O6 Ca O9 108.69(9) . . ?
O7 Ca O9 70.16(10) 1_655 1_545 ?
O3 Ca O9 55.96(12) 1_545 1_545 ?
O3 Ca O9 128.78(13) 4_575 1_545 ?
O1 Ca O9 125.62(13) 3_666 1_545 ?
O1 Ca O9 55.43(12) 2_646 1_545 ?
O5 Ca O9 110.41(10) . 1_545 ?
O6 Ca O9 108.69(9) . 1_545 ?
O9 Ca O9 135.34(19) . 1_545 ?
O7 Ca Si2 67.08(5) 1_655 . ?
O3 Ca Si2 102.36(9) 1_545 . ?
O3 Ca Si2 27.07(8) 4_575 . ?
O1 Ca Si2 80.45(9) 3_666 . ?
O1 Ca Si2 154.79(10) 2_646 . ?
O5 Ca Si2 111.69(5) . . ?
O6 Ca Si2 85.34(6) . . ?
O9 Ca Si2 29.18(9) . . ?
O9 Ca Si2 136.08(10) 1_545 . ?
O7 Ca Si2 67.08(5) 1_655 1_545 ?
O3 Ca Si2 27.08(8) 1_545 1_545 ?
O3 Ca Si2 102.36(9) 4_575 1_545 ?
O1 Ca Si2 154.79(10) 3_666 1_545 ?
O1 Ca Si2 80.45(9) 2_646 1_545 ?
O5 Ca Si2 111.69(5) . 1_545 ?
O6 Ca Si2 85.34(6) . 1_545 ?
O9 Ca Si2 136.08(10) . 1_545 ?
O9 Ca Si2 29.18(9) 1_545 1_545 ?
Si2 Ca Si2 118.93(6) . 1_545 ?
O7 Ca Si1 90.00(7) 1_655 3_666 ?
O3 Ca Si1 157.68(10) 1_545 3_666 ?
O3 Ca Si1 80.61(8) 4_575 3_666 ?
O1 Ca Si1 26.78(9) 3_666 3_666 ?
O1 Ca Si1 99.34(9) 2_646 3_666 ?
O5 Ca Si1 91.78(7) . 3_666 ?
O6 Ca Si1 117.04(4) . 3_666 ?
O9 Ca Si1 28.90(10) . 3_666 ?
O9 Ca Si1 133.99(10) 1_545 3_666 ?
Si2 Ca Si1 56.05(4) . 3_666 ?
Si2 Ca Si1 154.63(6) 1_545 3_666 ?
O4 Fe1 O4 180.0 . 3_666 ?
O4 Fe1 O1 87.74(17) . . ?
O4 Fe1 O1 92.25(17) 3_666 . ?
O4 Fe1 O1 92.26(17) . 3_666 ?
O4 Fe1 O1 87.75(17) 3_666 3_666 ?
O1 Fe1 O1 180.00(19) . 3_666 ?
O4 Fe1 O5 94.67(14) . . ?
O4 Fe1 O5 85.33(14) 3_666 . ?
O1 Fe1 O5 89.97(16) . . ?
O1 Fe1 O5 90.03(16) 3_666 . ?
O4 Fe1 O5 85.33(14) . 3_666 ?
O4 Fe1 O5 94.67(14) 3_666 3_666 ?
O1 Fe1 O5 90.03(16) . 3_666 ?
O1 Fe1 O5 89.97(16) 3_666 3_666 ?
O5 Fe1 O5 180.0(3) . 3_666 ?
O4 Fe1 Fe1 40.61(11) . 2_656 ?
O4 Fe1 Fe1 139.39(11) 3_666 2_656 ?
O1 Fe1 Fe1 91.65(10) . 2_656 ?
O1 Fe1 Fe1 88.35(10) 3_666 2_656 ?
O5 Fe1 Fe1 135.08(9) . 2_656 ?
O5 Fe1 Fe1 44.92(9) 3_666 2_656 ?
O4 Fe1 Fe1 139.39(11) . 2_646 ?
O4 Fe1 Fe1 40.61(11) 3_666 2_646 ?
O1 Fe1 Fe1 88.35(10) . 2_646 ?
O1 Fe1 Fe1 91.65(10) 3_666 2_646 ?
O5 Fe1 Fe1 44.92(9) . 2_646 ?
O5 Fe1 Fe1 135.08(9) 3_666 2_646 ?
Fe1 Fe1 Fe1 180.0 2_656 2_646 ?
O4 Fe1 Ce 88.76(14) . 3_666 ?
O4 Fe1 Ce 91.24(14) 3_666 3_666 ?
O1 Fe1 Ce 43.26(10) . 3_666 ?
O1 Fe1 Ce 136.74(10) 3_666 3_666 ?
O5 Fe1 Ce 133.00(13) . 3_666 ?
O5 Fe1 Ce 47.00(13) 3_666 3_666 ?
Fe1 Fe1 Ce 65.299(9) 2_656 3_666 ?
Fe1 Fe1 Ce 114.701(9) 2_646 3_666 ?
O10 Fe2 O11 179.63(18) . 1_545 ?
O10 Fe2 O3 88.33(17) . 1_545 ?
O11 Fe2 O3 91.45(17) 1_545 1_545 ?
O10 Fe2 O13 91.67(17) . 4_565 ?
O11 Fe2 O13 88.55(17) 1_545 4_565 ?
O3 Fe2 O13 179.43(17) 1_545 4_565 ?
O10 Fe2 O6 82.59(15) . . ?
O11 Fe2 O6 97.11(15) 1_545 . ?
O3 Fe2 O6 90.29(17) 1_545 . ?
O13 Fe2 O6 90.27(17) 4_565 . ?
O10 Fe2 O12 96.94(15) . 1_545 ?
O11 Fe2 O12 83.36(15) 1_545 1_545 ?
O3 Fe2 O12 91.53(17) 1_545 1_545 ?
O13 Fe2 O12 87.91(17) 4_565 1_545 ?
O6 Fe2 O12 178.1(2) . 1_545 ?
O10 Fe2 Fe2 139.48(11) . 4 ?
O11 Fe2 Fe2 40.79(11) 1_545 4 ?
O3 Fe2 Fe2 87.60(11) 1_545 4 ?
O13 Fe2 Fe2 92.03(11) 4_565 4 ?
O6 Fe2 Fe2 137.70(10) . 4 ?
O12 Fe2 Fe2 42.95(10) 1_545 4 ?
O10 Fe2 Fe2 40.52(11) . 4_565 ?
O11 Fe2 Fe2 139.21(11) 1_545 4_565 ?
O3 Fe2 Fe2 92.40(11) 1_545 4_565 ?
O13 Fe2 Fe2 87.97(11) 4_565 4_565 ?
O6 Fe2 Fe2 42.30(10) . 4_565 ?
O12 Fe2 Fe2 137.05(10) 1_545 4_565 ?
Fe2 Fe2 Fe2 180.0 4 4_565 ?
O10 Fe2 Ca 84.89(13) . . ?
O11 Fe2 Ca 94.75(13) 1_545 . ?
O3 Fe2 Ca 36.52(11) 1_545 . ?
O13 Fe2 Ca 144.04(12) 4_565 . ?
O6 Fe2 Ca 53.78(14) . . ?
O12 Fe2 Ca 128.05(14) 1_545 . ?
Fe2 Fe2 Ca 113.50(2) 4 . ?
Fe2 Fe2 Ca 66.50(2) 4_565 . ?
O8 Fe3 O4 166.8(2) 1_455 . ?
O8 Fe3 O2 81.55(13) 1_455 . ?
O4 Fe3 O2 89.47(13) . . ?
O8 Fe3 O2 81.55(13) 1_455 4_575 ?
O4 Fe3 O2 89.47(13) . 4_575 ?
O2 Fe3 O2 93.69(18) . 4_575 ?
O8 Fe3 O1 110.85(14) 1_455 . ?
O4 Fe3 O1 78.70(14) . . ?
O2 Fe3 O1 90.60(12) . . ?
O2 Fe3 O1 167.38(13) 4_575 . ?
O8 Fe3 O1 110.85(14) 1_455 4_575 ?
O4 Fe3 O1 78.70(14) . 4_575 ?
O2 Fe3 O1 167.38(13) . 4_575 ?
O2 Fe3 O1 90.60(12) 4_575 4_575 ?
O1 Fe3 O1 82.85(17) . 4_575 ?
O8 Fe3 Ce4 65.88(15) 1_455 . ?
O4 Fe3 Ce4 100.94(15) . . ?
O2 Fe3 Ce4 47.95(9) . . ?
O2 Fe3 Ce4 47.95(9) 4_575 . ?
O1 Fe3 Ce4 138.40(9) . . ?
O1 Fe3 Ce4 138.40(9) 4_575 . ?
O8 Fe3 Ce 108.87(16) 1_455 3_666 ?
O4 Fe3 Ce 84.31(15) . 3_666 ?
O2 Fe3 Ce 132.81(9) . 3_666 ?
O2 Fe3 Ce 132.81(9) 4_575 3_666 ?
O1 Fe3 Ce 42.30(9) . 3_666 ?
O1 Fe3 Ce 42.30(9) 4_575 3_666 ?
Ce4 Fe3 Ce 174.75(4) . 3_666 ?
O7 Si1 O9 107.5(3) . 3_666 ?
O7 Si1 O1 110.95(16) . 4_565 ?
O9 Si1 O1 106.64(16) 3_666 4_565 ?
O7 Si1 O1 110.95(16) . . ?
O9 Si1 O1 106.65(16) 3_666 . ?
O1 Si1 O1 113.8(3) 4_565 . ?
O7 Si1 Ce 116.47(7) . 3_666 ?
O9 Si1 Ce 66.07(8) 3_666 3_666 ?
O1 Si1 Ce 131.99(14) 4_565 3_666 ?
O1 Si1 Ce 41.19(12) . 3_666 ?
O7 Si1 Ce 116.47(7) . 3_656 ?
O9 Si1 Ce 66.07(8) 3_666 3_656 ?
O1 Si1 Ce 41.19(12) 4_565 3_656 ?
O1 Si1 Ce 131.99(14) . 3_656 ?
Ce Si1 Ce 116.14(6) 3_666 3_656 ?
O7 Si1 Ce 34.72(18) . 1_455 ?
O9 Si1 Ce 72.80(19) 3_666 1_455 ?
O1 Si1 Ce 121.95(13) 4_565 1_455 ?
O1 Si1 Ce 121.96(13) . 1_455 ?
Ce Si1 Ce 101.79(4) 3_666 1_455 ?
Ce Si1 Ce 101.79(4) 3_656 1_455 ?
O8 Si2 O3 108.95(16) . 4_575 ?
O8 Si2 O3 108.95(16) . . ?
O3 Si2 O3 112.2(2) 4_575 . ?
O8 Si2 O9 110.6(3) . . ?
O3 Si2 O9 108.09(16) 4_575 . ?
O3 Si2 O9 108.08(16) . . ?
O8 Si2 Ca 116.66(6) . . ?
O3 Si2 Ca 41.20(12) 4_575 . ?
O3 Si2 Ca 132.64(14) . . ?
O9 Si2 Ca 67.61(8) . . ?
O8 Si2 Ce 116.66(6) . 1_565 ?
O3 Si2 Ce 132.64(14) 4_575 1_565 ?
O3 Si2 Ce 41.20(12) . 1_565 ?
O9 Si2 Ce 67.61(8) . 1_565 ?
Ca Si2 Ce 118.93(6) . 1_565 ?
O8 Si2 Ce2 59.39(6) . 1_565 ?
O3 Si2 Ce2 137.22(14) 4_575 1_565 ?
O3 Si2 Ce2 50.80(12) . 1_565 ?
O9 Si2 Ce2 114.53(9) . 1_565 ?
Ca Si2 Ce2 175.81(5) . 1_565 ?
Ce Si2 Ce2 65.16(2) 1_565 1_565 ?
O8 Si2 Ce2 59.39(6) . . ?
O3 Si2 Ce2 50.80(12) 4_575 . ?
O3 Si2 Ce2 137.22(14) . . ?
O9 Si2 Ce2 114.53(9) . . ?
Ca Si2 Ce2 65.16(2) . . ?
Ce Si2 Ce2 175.81(5) 1_565 . ?
Ce2 Si2 Ce2 110.74(5) 1_565 . ?
O2 Si3 O2 103.7(3) . 4_565 ?
O2 Si3 O6 112.81(15) . . ?
O2 Si3 O6 112.81(15) 4_565 . ?
O2 Si3 O5 113.08(16) . . ?
O2 Si3 O5 113.09(16) 4_565 . ?
O6 Si3 O5 101.7(2) . . ?
O2 Si3 Ce2 51.91(13) . 1_455 ?
O2 Si3 Ce2 51.91(13) 4_565 1_455 ?
O6 Si3 Ce2 132.07(17) . 1_455 ?
O5 Si3 Ce2 126.20(18) . 1_455 ?
O2 Si3 Ca 127.88(13) . . ?
O2 Si3 Ca 127.88(13) 4_565 . ?
O6 Si3 Ca 57.50(16) . . ?
O5 Si3 Ca 44.23(17) . . ?
Ce2 Si3 Ca 170.43(6) 1_455 . ?
O14 Si4 O14 104.4(3) 1_565 4_565 ?
O14 Si4 O15 100.0(3) 1_565 4_575 ?
O14 Si4 O15 123.5(3) 4_565 4_575 ?
O14 Si4 O15 123.5(3) 1_565 . ?
O14 Si4 O15 100.0(3) 4_565 . ?
O15 Si4 O15 27.7(5) 4_575 . ?
O14 Si4 O12 112.09(16) 1_565 . ?
O14 Si4 O12 112.09(16) 4_565 . ?
O15 Si4 O12 104.2(3) 4_575 . ?
O15 Si4 O12 104.2(3) . . ?
O14 Si4 Ce3 127.60(13) 1_565 3_665 ?
O14 Si4 Ce3 127.60(13) 4_565 3_665 ?
O15 Si4 Ce3 48.5(2) 4_575 3_665 ?
O15 Si4 Ce3 48.5(2) . 3_665 ?
O12 Si4 Ce3 57.72(16) . 3_665 ?
O14 Si4 Ce4 52.81(13) 1_565 1_655 ?
O14 Si4 Ce4 52.81(13) 4_565 1_655 ?
O15 Si4 Ce4 117.0(2) 4_575 1_655 ?
O15 Si4 Ce4 117.0(2) . 1_655 ?
O12 Si4 Ce4 137.40(18) . 1_655 ?
Ce3 Si4 Ce4 164.88(6) 3_665 1_655 ?
O14 Si4 Ce3 42.38(13) 1_565 1_565 ?
O14 Si4 Ce3 123.75(14) 4_565 1_565 ?
O15 Si4 Ce3 57.7(2) 4_575 1_565 ?
O15 Si4 Ce3 81.8(2) . 1_565 ?
O12 Si4 Ce3 121.94(5) . 1_565 ?
Ce3 Si4 Ce3 95.45(4) 3_665 1_565 ?
Ce4 Si4 Ce3 76.15(3) 1_655 1_565 ?
O14 Si4 Ce3 123.75(14) 1_565 . ?
O14 Si4 Ce3 42.38(13) 4_565 . ?
O15 Si4 Ce3 81.8(2) 4_575 . ?
O15 Si4 Ce3 57.7(2) . . ?
O12 Si4 Ce3 121.94(5) . . ?
Ce3 Si4 Ce3 95.45(4) 3_665 . ?
Ce4 Si4 Ce3 76.15(3) 1_655 . ?
Ce3 Si4 Ce3 109.98(5) 1_565 . ?
O16 Si5 O17 110.4(3) . . ?
O16 Si5 O13 108.81(18) . 4_565 ?
O17 Si5 O13 108.13(16) . 4_565 ?
O16 Si5 O13 108.81(18) . . ?
O17 Si5 O13 108.13(16) . . ?
O13 Si5 O13 112.6(2) 4_565 . ?
O16 Si5 Ce3 68.7(3) . 1_455 ?
O17 Si5 Ce3 41.72(19) . 1_455 ?
O13 Si5 Ce3 122.55(12) 4_565 1_455 ?
O13 Si5 Ce3 122.56(12) . 1_455 ?
O16 Si5 Ce4 112.54(12) . 1_545 ?
O17 Si5 Ce4 58.71(6) . 1_545 ?
O13 Si5 Ce4 51.29(12) 4_565 1_545 ?
O13 Si5 Ce4 138.60(14) . 1_545 ?
Ce3 Si5 Ce4 75.88(3) 1_455 1_545 ?
O16 Si5 Ce4 112.54(12) . . ?
O17 Si5 Ce4 58.71(6) . . ?
O13 Si5 Ce4 138.60(14) 4_565 . ?
O13 Si5 Ce4 51.28(12) . . ?
Ce3 Si5 Ce4 75.88(3) 1_455 . ?
Ce4 Si5 Ce4 111.55(5) 1_545 . ?
Si1 O1 Fe1 124.7(2) . . ?
Si1 O1 Fe3 124.60(19) . . ?
Fe1 O1 Fe3 90.18(13) . . ?
Si1 O1 Ce 112.03(18) . 3_666 ?
Fe1 O1 Ce 101.61(14) . 3_666 ?
Fe3 O1 Ce 98.48(13) . 3_666 ?
Si3 O2 Fe3 125.95(18) . . ?
Si3 O2 Ce4 130.34(18) . . ?
Fe3 O2 Ce4 92.39(12) . . ?
Si3 O2 Ce2 99.32(16) . 1_455 ?
Fe3 O2 Ce2 106.50(12) . 1_455 ?
Ce4 O2 Ce2 97.73(10) . 1_455 ?
Si2 O3 Fe2 125.2(2) . 1_565 ?
Si2 O3 Ce 111.73(17) . 1_565 ?
Fe2 O3 Ce 114.94(16) 1_565 1_565 ?
Si2 O3 Ce2 101.94(15) . 1_565 ?
Fe2 O3 Ce2 104.08(14) 1_565 1_565 ?
Ce O3 Ce2 91.27(11) 1_565 1_565 ?
Fe1 O4 Fe1 98.8(2) 2_656 . ?
Fe1 O4 Fe3 102.14(18) 2_656 . ?
Fe1 O4 Fe3 102.14(18) . . ?
Si3 O5 Fe1 128.31(14) . . ?
Si3 O5 Fe1 128.31(14) . 2_646 ?
Fe1 O5 Fe1 90.17(18) . 2_646 ?
Si3 O5 Ca 108.4(2) . . ?
Fe1 O5 Ca 97.16(15) . . ?
Fe1 O5 Ca 97.16(15) 2_646 . ?
Si3 O6 Fe2 131.60(11) . . ?
Si3 O6 Fe2 131.60(11) . 4_565 ?
Fe2 O6 Fe2 95.4(2) . 4_565 ?
Si3 O6 Ca 93.95(19) . . ?
Fe2 O6 Ca 93.68(15) . . ?
Fe2 O6 Ca 93.68(15) 4_565 . ?
Si1 O7 Ce 122.6(3) . 1_455 ?
Si1 O7 Ce2 135.3(3) . 1_455 ?
Ce O7 Ce2 102.15(18) 1_455 1_455 ?
Si2 O8 Fe3 129.5(3) . 1_655 ?
Si2 O9 Si1 148.7(4) . 3_666 ?
Si2 O9 Ca 83.21(11) . . ?
Si1 O9 Ca 85.03(12) 3_666 . ?
Fe2 O10 Fe2 99.0(2) 4_565 . ?
Fe2 O10 Ce2 106.82(15) 4_565 . ?
Fe2 O10 Ce2 106.82(15) . . ?
Fe2 O10 H1 111(3) 4_565 . ?
Fe2 O10 H1 111(3) . . ?
Ce2 O10 H1 121(6) . . ?
Fe2 O11 Fe2 98.4(2) 4_565 1_565 ?
Fe2 O11 Ce4 107.28(15) 4_565 . ?
Fe2 O11 Ce4 107.28(15) 1_565 . ?
Fe2 O11 H2 120(3) 4_565 . ?
Fe2 O11 H2 120(3) 1_565 . ?
Ce4 O11 H2 103(5) . . ?
Si4 O12 Fe2 130.42(12) . 1_565 ?
Si4 O12 Fe2 130.42(12) . 4_565 ?
Fe2 O12 Fe2 94.1(2) 1_565 4_565 ?
Si4 O12 Ce3 92.0(2) . 3_665 ?
Fe2 O12 Ce3 100.74(15) 1_565 3_665 ?
Fe2 O12 Ce3 100.74(15) 4_565 3_665 ?
Si5 O13 Fe2 123.6(2) . 4_565 ?
Si5 O13 Ce3 114.83(17) . 3_665 ?
Fe2 O13 Ce3 110.77(15) 4_565 3_665 ?
Si5 O13 Ce4 101.01(15) . . ?
Fe2 O13 Ce4 101.56(14) 4_565 . ?
Ce3 O13 Ce4 100.39(11) 3_665 . ?
Si4 O14 Ce2 135.78(19) 1_545 . ?
Si4 O14 Ce3 112.25(19) 1_545 . ?
Ce2 O14 Ce3 100.52(13) . . ?
Si4 O14 Ce4 98.29(16) 1_545 1_645 ?
Ce2 O14 Ce4 99.33(12) . 1_645 ?
Ce3 O14 Ce4 107.38(12) . 1_645 ?
O15 O15 Si4 76.1(2) 4_575 . ?
O15 O15 Ce3 81.12(15) 4_575 3_665 ?
Si4 O15 Ce3 102.6(3) . 3_665 ?
O15 O15 Ce3 146.53(13) 4_575 . ?
Si4 O15 Ce3 94.6(3) . . ?
Ce3 O15 Ce3 132.3(3) 3_665 . ?
Si5 O16 Ce4 179.2(4) . 3_565 ?
Si5 O17 Ce3 112.2(3) . 1_455 ?
Si5 O17 Ce4 93.82(11) . 1_545 ?
Ce3 O17 Ce4 102.02(10) 1_455 1_545 ?
Si5 O17 Ce4 93.82(11) . . ?
Ce3 O17 Ce4 102.02(10) 1_455 . ?
Ce4 O17 Ce4 149.8(2) 1_545 . ?
 
loop_
 _geom_hbond_atom_site_label_D 
 _geom_hbond_atom_site_label_H 
 _geom_hbond_atom_site_label_A 
 _geom_hbond_distance_DH 
 _geom_hbond_distance_HA 
 _geom_hbond_distance_DA 
 _geom_hbond_angle_DHA 
 _geom_hbond_site_symmetry_A 
 _geom_hbond_publ_flag
O10 H1 O15  0.850(10) 1.878(18) 2.706(8) 165(5) 3_665 yes
O10 H1 O15  0.850(10) 1.878(18) 2.706(8) 165(5) 2_645 yes
O11 H2 O4  0.850(10) 2.096(14) 2.944(7) 175(8) . yes
 
_refine_diff_density_max    2.210
_refine_diff_density_min   -2.279
_refine_diff_density_rms    0.220



